Experimental and theoretical studies of structural phase transition in a novel polar perovskite-like [C2H5NH3][Na0.5Fe0.5(HCOO)3] formate.
Ptak, Maciej; Mączka, Mirosław; Gągor, Anna; Sieradzki, Adam; Stroppa, Alessandro; Di Sante, Domenico; Perez-Mato, Juan Manuel; Macalik, Lucyna; Dalton transactions (Cambridge, England : 2003) 45 (2016) 2574–2583; doi:10.1039/c5dt04536c

data_7037688
_publ_section_title
;
 Experimental and theoretical studies of structural phase transition in a
 novel polar perovskite-like [C2H5NH3][Na0.5Fe0.5(HCOO)3] formate.
;
_journal_issue                   6
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              2574
_journal_page_last               2583
_journal_paper_doi               10.1039/c5dt04536c
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'C10 H22 Fe N2 Na O12'
_chemical_formula_weight         441.13
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-11-12 deposited with the CCDC.
2015-12-16 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 91.125(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.1102(2)
_cell_length_b                   9.3794(4)
_cell_length_c                   12.1341(4)
_cell_measurement_reflns_used    1940
_cell_measurement_temperature    377(2)
_cell_measurement_theta_max      27.3610
_cell_measurement_theta_min      2.8180
_cell_volume                     922.85(5)
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      377(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Xcalibur, Sapphire1, long nozzle'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0206
_diffrn_reflns_av_unetI/netI     0.0298
_diffrn_reflns_laue_measured_fraction_full 0.993
_diffrn_reflns_laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            3623
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.682
_diffrn_reflns_theta_max         25.682
_diffrn_reflns_theta_min         3.049
_exptl_absorpt_coefficient_mu    0.902
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.97633
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35h (release 09-02-2015 CrysAlis171 .NET)
(compiled Feb  9 2015,16:26:32)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    1.588
_exptl_crystal_description       prism
_exptl_crystal_F_000             458
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.205
_refine_diff_density_min         -0.230
_refine_diff_density_rms         0.051
_refine_ls_extinction_coef       0.015(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.204
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     150
_refine_ls_number_reflns         1737
_refine_ls_number_restraints     42
_refine_ls_restrained_S_all      1.208
_refine_ls_R_factor_all          0.0502
_refine_ls_R_factor_gt           0.0425
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0300P)^2^+0.7600P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0962
_refine_ls_wR_factor_ref         0.0994
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1519
_reflns_number_total             1737
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5dt04536c2.cif
_cod_data_source_block           377K
_cod_depositor_comments
'Adding full bibliography for 7037687--7037688.cif.'
_cod_original_cell_volume        922.85(6)
_cod_database_code               7037688
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              93272
_shelx_hkl_checksum              67107